The lateral resistance of dowel-type connections with CLT is related to its lay-up, species of the laminations and even the manufacture method. Treating the CLT as homogeneous material, current methods develop new equations through test results or make use of the existing equations for the embedment strength already used in design codes; thus, the lateral resistance of dowel-type connections of CLT can be calculated. This kind of approach does not take the embedment stress distribution into account, which may lead to inaccuracy in predicting the lateral resistance and yield mode of the dowel-type connections in CLT. In this study, tests of the bolted connections and the screwed connections of CLT were conducted by considering the effects of the orientation of the laminations, the thickness of the connected members, the fastener diameter and strength of the materials. The material properties including yield strength of the fasteners and embedment strength of the CLT laminations were also tested. Using analysis of the dowel-type connections of CLT by introducing the equivalent embedment stress distribution, equations for the lateral resistance of the connections based on the European Yield Model were developed. The predicted lateral resistance and yield modes were in good agreement with the test results; the correctness and the feasibility of the equations were thus validated.
Process parameters of cross-laminated timber (CLT) fabricated with Japanese larch were evaluated. The process parameters were designed by using an orthogonal test including pressure, glue consumption, and adhesive. Both delamination and block shear tests were conducted on CLT in accordance with GB/T 26899 (2011). The results showed that the optimum process parameters were A2B3C2 including pressure (1.2 MPa), glue consumption (200g/m2), and amount of sdhesive (one-component plyurethane). The weight loss and moisture absoption increased when the temperature increased, but the block shear strength decreased as the temperature was raised from 20C to 230C.